The emergence of exotic quantum phenomena is often triggered by a subtle change in the crystal phase. Transition metal dichalcogenides (TMDs) exhibit a wide variety of novel properties, depending on their crystal phases, which can be trigonal prismatic (2H) or octahedral (1T). Bulk NbSe2 crystallizes into the 2H phase, and the charge density wave and the superconductivity emerge simultaneously and interact with each other, thereby creating various anomalous properties. However, these properties and their interplay in another polymorph, 1T-NbSe2, have remained unclear because of the difficulty of synthesizing it. Here we report the first experimental realization of a monolayer 1T-NbSe2 crystal grown epitaxially on bilayer graphene. In contrast with 2H-NbSe2, monolayer 1T-NbSe2 was found to be a Mott insulator, with an energy gap of 0.4 eV. We also found that the insulating 1T and metallic 2H phases can be selectively fabricated by simply controlling the substrate temperature during epitaxy. The present results open a path to crystal-phase engineering based on TMDs.
Atomic-layer materials have recently attracted attention, because they exhibit a variety of anomalous properties distinct from those of their three-dimensional bulk counterparts, as exemplified by the Dirac-cone states in graphene1 and the high-temperature superconductivity in ultrathin iron-based superconductor films.2 Whereas atomic-layer materials are inherently unstable, owing to their tendency to progress toward long-range order,3 such characteristics may facilitate the exploration of new crystal phases that cannot usually be realized in bulk. For instance, the local crystal structure at the surfaces of transition metal dichalcogenides (TMDs) is known to be sensitive to crystal defects, chemical reactions and thermal effects,4, 5, 6, 7, 8, 9 thus suggesting the feasibility of crystal-phase control in two dimension. The structural transition between 2H- (trigonal prismatic structure, D3h) and 1T- (octahedral structure, Oh) polymorphs (see Figure 1a) in monolayer MoS2 is a typical example that cannot be achieved in the bulk phase.5, 6, 7 Bulk NbSe2 has several polymorphs: 3R, 4H and 2H, although the essential structural unit is identical, trigonal prismatic. Here we term a monolayer consisting of this structural unit 2H-NbSe2.
Among TMDs, bulk 2H-NbSe2 has been the target of intensive studies, because it exhibits a unique ground state in which an incommensurate charge density wave (CDW) and superconductivity coexist below 7 K.10 Recent success in fabricating monolayer and multilayer 2H-NbSe2 films has revealed drastic changes in the superconducting and CDW transition temperatures with changes in the number of layers, thus providing a valuable opportunity for studying key questions regarding the interplay among dimensionality, the CDW and superconductivity.11, 12, 13, 14 In contrast to the intensively studied 2H-NbSe2,15, 16 the 1T counterpart has not yet been synthesized either in bulk or as an ultrathin film. Although a 1T-like phase has been observed locally around defects17, 18, 19 in thermally treated bulk samples,20 AgxNb2Se3 (Koslowski et al.21) and Nb1−xTixSe2 (Di Salvo et al.22), it has been difficult to selectively fabricate a pristine sample of a single phase for precise physical measurements as well as for device applications. It is thus of great importance to fabricate an ultrathin film of pristine 1T-NbSe2 and to investigate its electronic states to reveal as-yet-unknown electronic properties. Here, combining molecular-beam epitaxy and state-of-the-art electron spectroscopy methods, we succeeded in selectively fabricating 1T and 2H single-phase monolayer NbSe2 on bilayer graphene and investigated the anomalous electronic states in detail.
Materials and methods
A monolayer NbSe2 film was grown on bilayer graphene by using molecular-beam epitaxy in ultrahigh vacuum (3 × 10−10 Torr). Bilayer graphene was prepared by annealing an n-type Si-rich 6H-SiC(0001) single-crystal wafer,23, 24 by resistive heating at 1100 °C in high vacuum—better than 1.0 × 10−9Torr—for 20 min. A monolayer NbSe2 film was grown by evaporating Nb on the bilayer graphene substrate in a Se atmosphere. The substrate was kept at 500–590 °C during epitaxy. The as-grown film was annealed at 400 °C for 30 min and then transferred to the angle-resolved photoemission spectroscopy (ARPES)-measurement chamber without breaking vacuum. The growth process was monitored by reflection high-energy electron diffraction. The custom-made scanning tunneling microscopy (STM) system was operated at T=4–6 K under ultrahigh vacuum (below 2 × 10−10 Torr). The ARPES measurements were carried out using an MBS-A1 (MB Scientific AB, Uppsala, Sweden) electron-energy analyzer with a high-flux helium discharge lamp and a toroidal grating monochromator at Tohoku University. The energy and angular resolutions were set at 16 meV and 0.2º, respectively. The Fermi level (EF) of samples was calibrated with a gold film deposited onto the substrate. First-principles band-structure calculations for free-standing 2H- and 1T-NbSe2 monolayers were carried out by using the Quantum Espresso code.25 Spin–orbit interactions were included in the calculations. The plane-wave cutoff energy and the k-point mesh were set to be 30 Ry and 12 × 12 × 1, respectively. The thickness of the inserted vacuum layer in a model crystal was set to ~10 Å.
Results and discussion
We used the van der Waals epitaxy technique26 to fabricate monolayer NbSe2 (Ugeda et al.13) by using bilayer graphene grown on silicon carbide as a substrate. Figure 1b shows the reflection high-energy electron diffraction pattern of bilayer graphene on 6H-SiC(0001), which signified a 1 × 1 streak pattern and spots originating from the bilayer graphene and the buffer layer beneath it, respectively.23, 24 After co-evaporation of Nb and Se atoms onto a substrate kept at 530 °C in ultrahigh vacuum, the reflection high-energy electron diffraction intensity of spots was reduced and a new 1 × 1 pattern appeared (Figure 1c). This behavior is characteristic of a TMD ultrathin film, as has been observed in monolayer WSe2 and TiSe2 on bilayer graphene.23, 24 STM revealed the formation of monolayer NbSe2 islands (Figure 1d), whose height (~ 0.7 nm; see line profile in Figure 1e) was nearly equal to the distance between adjacent NbSe2 layers in bulk 2H-NbSe2, 0.63 Å.10 We found that this film was composed of two different types of islands. One, called type-A here, exhibited a 1 × 1 atomic structure (Figure 1f), whereas the other, type-B, showed no clear atomic order. The former islands showed characteristic V-shaped density of states with a finite density of states at zero-bias voltage in the dI/dV curve at T=6 K, a result reminiscent of the spectral features of bulk 2H-NbSe2.18 This island type is probably made of 2H domains. However, the dI/dV curve of type-B islands showed markedly different characteristics; the density of states vanished in a wide energy region of ±0.2 eV with respect to EF, indicating an insulating nature with an energy gap of ~0.4 eV. These results demonstrated that both metallic and insulating crystal phases coexisted in this monolayer NbSe2 film.
To further clarify the nature of the two different islands, we performed ARPES on this film. It was expected that the characteristic spectral features from both domains would be simultaneously observed in an ARPES spectrum, because this technique probes a relatively large surface area (~2 × 2 mm2). As shown in Figure 2a, the ARPES-intensity plot along the ΓM cut resolved several dispersive bands in the valence band region, reflecting the high single-crystallinity of the film. Figure 2b shows the valence-band ARPES-intensity plot of bulk 2H-NbSe2, which is useful for distinguishing the contribution of the 2H phase in a monolayer film, because the overall experimental valence band dispersion in this wide energy range is known to be similar between the bulk and the monolayer.13, 15, 16 In previous studies, the band calculations have revealed several differences in the band dispersions near EF between the bulk and the monolayer, such as the presence or absence of the kz dispersion in the Nb 4d band and the EF crossing or non-crossing of the anti-bonding Se pz band.13, 27 A side-by-side comparison of the ARPES-intensity plots in Figure 2a and b revealed that the observed band structures shared several common features, for example, the band near EF around the M point, which crosses EF midway between Γ and M, and the hole-like bands with the top of the dispersion at the binding energies (EB) of 0.9 and 1.2 eV at Γ, as highlighted by the blue dashed curves. In Figure 2c, some corresponding bands are visible in the calculated band structure for monolayer 2H-NbSe2, whereas several quantitative differences are also apparent in the energy of the bands (see, for example, the hole-like bands at EB~1 eV at Γ). In addition to the bands ascribed to the 2H phase, Figure 2a shows additional bands that are absent in bulk and monolayer 2H-NbSe2,13, 15, 16 such as a relatively flat feature at EB—0.4 eV around Γ (here denoted the α-band), a faint hole-like band at Γ (β-band) and a larger hole-like band (γ-band), as highlighted by the red dashed curves. These bands are likely to be of 1T phase in origin, because a corresponding feature in the calculated bands for monolayer 1T-NbSe2 (Figure 2c) is apparent, particularly in the β- and γ-bands. Intriguingly, although the calculations predict the EF crossings of hole-like bands around Γ, the ARPES intensity was strongly suppressed around EF, thus suggesting an opening of an energy gap. Apparently, this gap was not an ordinary band gap, because the first-principles calculation failed to reproduce it, as shown in Figure 2j, which highlights the essential difference between the experimental and the calculated band dispersions around EF. The opening of such an energy gap could not be explained in terms of carrier doping, because the band calculation for monolayer 1T-NbSe2 showed no band gap around the Γ point, irrespective of the location of the chemical potential (Figure 2c). Instead, the observed gap may have arisen from a Mott–Hubbard gap, because the similar material bulk 1T-TaSe2 shows almost identical band dispersions in the Mott phase.28, 29, 30 In this context, the α-band was assigned to the lower Hubbard band. Moreover, the insulating type-B islands in the STM image probably arose from the 1T phase, taking into account the similar energy scales for the gap below EF found by ARPES and STM (~0.25 eV), as seen from a comparison of Figures 1h and 2j.
Having established the existence of a 1T/2H-mixed phase in monolayer NbSe2, we next addressed how to selectively fabricate these two phases. We found that the temperature of the bilayer graphene substrate (TS) during the epitaxy of the NbSe2 film was a major parameter controlling the crystal phase. Whereas the mixed phase presented in Figures 1 and 2a was obtained at TS=530 °C, we found that the 2H (1T) single phase was obtained at a slightly lower (higher) TS. As evident from Figure 2d and e, which show the ARPES intensities for the 2H phase (TS=515 °C), no obvious mixture of the 1T-phase bands was observed (compared with Figure 2a and d). Similarly, the ARPES intensity for the 1T phase (TS=590 °C) showed negligible contamination from the 2H phase, as evident from the absence of EF crossing bands, as shown in Figure 2i and j. This selective fabrication of the 2H and 1T phases is also highlighted in Figure 2f and k, which show that the Fermi surface (FS) of the 2H phase consisted of a large hexagonal pocket at Γ and another large pocket at K (Figure 2f), as in the bulk sample,15, 16 whereas the FS was completely absent in the 1T phase, as seen from the featureless intensity pattern at EF (Figure 2k). The control of crystal phases via temperature has been used in the chemical vapor transport method to obtain 1T and 2H phases in some bulk TMDs.31, 32, 33 Our results thus suggest that temperature control is a key factor for obtaining different crystal phases in both monolayer and bulk TMDs.
The selective fabrication of 1T and 2H phases was further corroborated by our STM measurements. We found that the 1T phase (Ts=590 °C) consisted of several monolayer 1T islands on the graphene substrate (Figure 2l), unlike the 2H counterpart, which appeared to grow layer by layer, as inferred from its large terrace size (Figure 2g). Intriguingly, closer examination of one of the 1T islands in Figure 2m revealed the modulation of density of states with periodicity (note that this modulation is not clearly resolved in the 1T/2H-mixed phase in Figure 1g, probably because of the low film quality). This result strongly suggests the formation of ‘star-of-David’ clusters, similar to the case of the Mott-insulating (commensurate CDW) phases of bulk 1T-TaS2 and TaSe2,28, 30, 34 thus supporting the Mott-insulating nature of the 1T phase. In contrast, the STM image of the 2H counterpart showed a 3 × 3 intensity modulation (Figure 2h), which followed the periodicity of the CDW in bulk and monolayer 2H-NbSe2.13, 26 These STM results, together with the ARPES results, firmly establish the intrinsic differences between the electronic states of the 1T and 2H phases.
To experimentally determine the temperature ranges suitable for the selective growth of pure 1T or 2H single phases, we performed systematic ARPES measurements for samples with various TS values. We evaluated the ratio of 1T and 2H components from the energy distribution curve along the ΓM cut on the hexagonal pocket, seen in the 2H phase (kx=0.5 Å−1). We numerically fit the energy distribution curve with two Lorentzian peaks originating from the 2H and 1T phases located at around 0 and 0.4 eV, respectively. In Figure 3b, the energy distribution curve for TS=515 °C showed a single peak at EF, thus supporting its purely 2H-phase nature. On increasing TS, the intensity of this peak was monotonically reduced, in accordance with the evolution of the 0.4 eV peak. This finding suggested that the ratio between the 1T and 2H phases systematically changes as a function of TS, as highlighted by the phase diagram in Figure 3a. We also found that TS values below 500 °C or above 600 °C were not suitable for the fabrication of monolayer NbSe2, owing to the presence of multiple 2H domains with unfixed axis orientations and/or the difficulty of maintaining a stable monolayer crystal phase. From this empirical evidence, together with the results of Figure 3a, we concluded that the TS values best suited for obtaining 2H or 1T single phases are 500–515 °C and 580–600 °C, respectively.
A previous study of monolayer 2H-NbSe2 (Ugeda et al.13) has suggested that two types of 2H domains, rotated by 30° with respect to each other, can exist when the film is fabricated at low TS (~330 °C). As described above, we found a way to selectively fabricate the single-domain 2H phase by keeping the TS above 500 °C. When two domains are mixed in a sample, the appearance of a complicated FS is expected. For example, besides the intrinsic FS at K, a replica FS should appear around M. In contrast, as shown in Figure 2d, our ARPES intensity mapping for the Ts=515 °C sample showed no signature of the FS at M, thereby strongly suggesting the single-domain nature of our 2H-phase sample. This conclusion is also supported by the experimental evidence that the FS at the Γ point exhibited a clear hexagonal shape consistent with the sixfold symmetry of a single domain.
The present success of the selective fabrication of insulating 1T and metallic 2H phases may contribute to realizing a field effect transistor based on semiconducting monolayer 1T-NbSe2 and metallic 2H-NbSe2. Although polymorph field effect transistors have recently been reported by using other TMDs such as MoS2 and MoTe2,8, 9 the unique Mott-insulating state of 1T-NbSe2, distinct from the states of the band-insulating 2H-MoS2 and 2H-MoTe2, would provide a new means of controlling a device, because the characteristics of the Mott-insulating state in the 1T phase are known to be altered by various physical parameters, such as pressure and disorder.34, 35 Furthermore, as monolayer 2H-NbSe2 exhibits superconductivity robust against magnetic fields owing to space inversion symmetry breaking and the resultant spin imbalance in the electronic states,12 the present result also opens a path toward atomic-layer electronics based on superconductor/semiconductor heterojunctions.
Novoselov, K. S., Geim, A. K., Morozov, S. V., Jiang, D., Katsnelson, M. I., Grigorieva, I. V., Dubonos, S. V. & Firsov, A. A. Two-dimensional gas of massless Dirac fermions in graphene. Nature 438, 197–200 (2005).
Wang, Q.-Y., Li, Z., Zhang, W.-H., Zhang, Z.-C., Zhang, J.-S., Li, W., Ding, H., Ou, Y.-B., Deng, P., Chang, K., Wen, J., Song, C.-L., He, K., Jia, J.-F., Ji, S.-H., Wang, Y.-Y., Wang, L.-L., Chen, X., Ma, X.-C. & Xue, Q.-K. Interface-induced high-temperature superconductivity in single unit-cell FeSe films on SrTiO3 . Chin. Phys. Lett. 29, 037402 (2012).
Mermin, N. D. Crystalline order in two dimensions. Phys. Rev. 176, 250–254 (1968).
Py, M. A. & Haering, R. R. Structural destabilization induced by lithium intercalation in MoS2 and related compounds. Can. J. Phys. 61, 76–84 (1983).
Kang, Y., Najmaei, S., Liu, Z., Bao, Y., Wang, Y., Zhu, X., Halas, N. J., Nordlander, P., Ajayan, P. M., Lou, J. & Fang, Z. Plasmonic hot electron induced structural phase transition in a MoS2 monolayer. Adv. Mater. 26, 6467–6471 (2014).
Lin, Y.-C., Dumcenco, D. O., Huang, Y.-S. & Suenaga, K. Atomic mechanism of the semiconducting-to-metallic phase transition in single-layered MoS2 . Nat. Nanotechnol. 9, 391–396 (2014).
Ambrosi, A., Sofer, Z. & Pumera, M. 2H→1 T phase transition and hydrogen evolution activity of MoS2, MoSe2, WS2 and WSe2 strongly depends on the MX2 composition. Chem. Commun. 51, 8450–8453 (2015).
Kappera, R., Voiry, D., Yalcin, S. E., Branch, B., Gupta, G., Mohite, A. D. & Chhowalla, M. Phase-engineered low-resistance contacts for ultrathin MoS2 transistors. Nat. Mater. 13, 1128–1134 (2014).
Cho, S., Kim, S., Kim, J. H., Zhao, J., Seok, J. D., Keum, H., Baik, J., Choe, D.-H., Chang, K. J., Suenaga, K., Kim, S. W., Lee, Y. H. & Yang, H. Phase patterning for ohmic homojunction contact in MoTe2 . Science 349, 625–628 (2015).
Wilson, J. A., Di Salvo, F. J. & Mahajan, S. Charge-density waves and superlattices in the metallic layered transition metal dichalcogenides. Adv. Phys. 24, 117–201 (1975).
Xi, X., Zhao, L., Wang, Z., Berger, H., Forró, L., Shan, J. & Mak., K. F. Strongly enhanced charge-density-wave order in monolayer NbSe2 . Nat. Nanotechnol. 10, 765–769 (2015).
Xi, X., Wang, Z., Zhao, W., Park, J.-H., Law, K. T., Berger, H., Forró, L., Shan, J. & Mak., K. F. Ising pairing in superconducting NbSe2 atomic layers. Nat. Phys. 12, 139–143 (2016).
Ugeda, M. M., Bradley, A. J., Zhang, Y., Onishi, S., Chen, Y., Ruan, W., Ojeda-Aristizabal, C., Ryu, H., Edmonds, M. T., Tsai, H.-Z., Riss, A., Mo, S.-K., Lee, D., Zettl, A., Hussain, Z., Shen, Z.-X. & Crommie, M. F. Characterization of collective ground states in single-layer NbSe2 . Nat. Phys. 12, 92–97 (2016).
Cao, Y., Mishchenko, A., Yu, G. L., Khestanova, E., Rooney, A. P., Prestat, E., Kretinin, A. V., Blake, P., Shalom, M. B., Woods, C., Chapman, J., Balakrishnan, G., Grigorieva, I. V., Novoselov, K. S., Piot, B. A., Potemski, M., Watanabe, K., Taniguchi, T., Haigh, S. J., Geim, A. K. & Gorbachev, R. V. Quality heterostructures from two-dimensional crystals unstable in air by their assembly in inert atmosphere. Nano Lett. 15, 4914–4921 (2015).
Yokoya, T., Kiss, T., Chainani, A., Shin, S., Nohara, M. & Takagi, H. Fermi surface sheet-dependent superconductivity in 2H-NbSe2 . Science 294, 2518–2520 (2001).
Rahn, D. J., Hellmann, S., Kalläne, M., Sohrt, C., Kim, T. K., Kipp, L. & Rossnagel, K. Gaps and kinks in the electronic structure of the superconductor 2H-NbSe2 from angle-resolved photoemission at 1 K. Phys. Rev. B 85, 224532 (2012).
Ramšak, N., van Midden, H. J. P., Prodan, A., Marinković, V., Boswell, F. W. & Bennett, J. C. Defect-induced room-temperature modulation in NbSe2 . Phys. Rev. B 60, 4513–4516 (1999).
Komori, F., Iwaki, T., Hattori, K., Shiino, O. & Hasegawa, T. New superstructure on the surface of 2H-NbSe2 and tunneling spectra at 4.2 K. J. Phys. Soc. Jpn 66, 298–301 (1997).
Wang, H., Lee, J., Dreyer, M. & Barker, B. I. A scanning tunneling microscopy study of a new superstructure around defects created by tip–sample interaction on 2H-NbSe2 . J. Phys. Condens. Matter 21, 265005 (2009).
Kadijk, F. & Jellinek, F. On the polymorphism of niobium diselenide. J. Less Common. Met. 23, 437–441 (1971).
Koslowski, B., Xu, W., Blackford, B. & Jericho, M. H. Observation of a superlattice in silver-intercalated NbSe2 by scanning tunneling microscopy. Phys. Rev. B 54, 11706–11709 (1996).
Di Salvo, F. J., Wilson, J. A., Bagley, B. G. & Waszczak, J. V. Effects of doping on charge-density waves in layer compounds. Phys. Rev. B 12, 2220–2236 (1975).
Sugawara, K., Sato, T., Tanaka, Y., Souma, S. & Takahashi., T. Spin- and valley- coupled electronic states in monolayer WSe2 on bilayer graphene. Appl. Phys. Lett. 107, 071601 (2015).
Sugawara, K., Nakata, Y., Shimizu, R., Patrick, H., Hitosugi, T., Sato, T. & Takahashi, T. Unconventional charge-density-wave transition in monolayer 1 T-TiSe2 . ACS Nano 10, 1341–1345 (2016).
Giannozzi, P., Baroni, S., Bonini, N., Calandra, M., Car, R., Cavazzoni, C., Ceresoli, D., Chiarotti, G. L., Cococcioni, M., Dabo, I., Corso, A. D., de Gironcoli, S., Fabris, S., Fratesi, G., Gebauer, R., Gerstmann, U., Gougoussis, C., Kokalj, A., Lazzeri, M., Martin-Samos, L., Marzari, N., Mauri, F., Mazzarello, R., Paolini, S., Pasquarello, A., Paulatto, L., Sbraccia, C., Scandolo, S., Sclauzero, G., Seitsonen, A. P., Smogunov, A., Umari, P. & Wentzcovitch, R. M. QUANTUM ESPRESSO: a modular and open-source software project for quantum simulations of materials. J. Phys. Condens. Matter 21, 395502 (2009).
Koma, A., Sunouchi, K. & Miyajima, T. Fabrication and characterization of heterostructures with subnanometer thickness. Microelectron. Eng. 2, 129–136 (1984).
Calandra, M., Mazin, I. I. & Mauri, F. Effect of dimensionality on the charge-density wave in few-layer 2H-NbSe2 . Phys. Rev. B 80, 241108(R) (2009).
Ang, R., Tanaka, Y., Ieki, E., Nakayama, K., Sato, T. L., Li, J., Lu, W. J., Sun, Y. P. & Takahashi, T. Real-space coexistence of the melted Mott state and superconductivity in Fe-substituted 1 T-TaS2 . Phys. Rev. Lett. 109, 176403 (2012).
Perfetti, L., Georges, A., Florens, S., Biermann, S., Mitrovic, S., Berger, H., Tomm, Y., Höchst, H. & Grioni, M. Spectroscopic signatures of a bandwidth-controlled Mott transition at the surface of 1 T-TaSe2 . Phys. Rev. Lett. 90, 166401 (2003).
Colonna, S., Ronci, F., Cricenti, A., Perfetti, L., Berger, H. & Grioni, M. Mott phase at the surface of 1 T-TaSe2 observed by scanning tunneling microscopy. Phys. Rev. Lett. 94, 036405 (2005).
Samnakay, R., Wickramaratne, D., Pope, T. R., Lake, R. K., Salguero, T. T. & Balandin, A. A. Zone-folded phonons and the commensurate–incommensurate charge-density-wave transition in 1 T-TaSe2 thin films. Nano Lett. 15, 2965–2973 (2015).
Renteria, J., Samnakay, R., Jiang, C., Pope, T. R., Goli, P., Yan, Z., Wickramaratne, D., Salguero, T. T., Khitun, A. G., Lake, R. K. & Balandin, A. A. All-metallic electrically gated 2H-TaSe2 thin-film switches and logic circuits. J. Appl. Phys. 115, 034305 (2014).
Yan, Z., Jiang, C., Pope, T. R., Tsang, C. F., Stickney, J. L., Goli, P., Renteria, J., Salguero, T. T. & Balandin, A. A. Phonon and thermal properties of exfoliated TaSe2 thin films. J. Appl. Phys. 114, 204301 (2013).
Sipos, B., Kusmartseva, A. F., Akrap, A., Berger, H., Forró, L. & Tutiš, E. From Mott state to superconductivity in 1 T-TaS2 . Nat. Mater. 7, 960–965 (2008).
Xu, P., Piatek, J. O., Lin, P.-H., Sipos, B., Berger, H., Forró, L., Rønnow, H. M. & Grioni, M. Superconducting phase in the layered dichalcogenide 1 T-TaS2 upon inhibition of the metal-insulator transition. Phys. Rev. B 81, 172503 (2010).
We thank K Yamada, H Kimizuka, N Shimamura, Y Tanaka and S Souma for their help with the ARPES experiments. We also thank T Koretsune for help with using the quantum ESPRESSO package. This work was supported by the JSPS KAKENHI Grant Numbers JP15H02105, JP25107003 and JP15H05853, the Program for Key Interdisciplinary Research and the World Premier International Research Center, Advanced Institute for Materials Research.
YN and KS carried out the fabrication of thin films, their characterization and the ARPES measurements. KU fabricated the bulk 2H-NbSe2 single crystals. KS performed the band calculations. RS, YO, PH and TH performed the STM experiments. YN, KS, TS and TT finalized the manuscript with input from all the authors.
The authors declare no conflict of interest.
Rights and permissions
This work is licensed under a Creative Commons Attribution 4.0 International License. The images or other third party material in this article are included in the article’s Creative Commons license, unless indicated otherwise in the credit line; if the material is not included under the Creative Commons license, users will need to obtain permission from the license holder to reproduce the material. To view a copy of this license, visit http://creativecommons.org/licenses/by/4.0/
About this article
Cite this article
Nakata, Y., Sugawara, K., Shimizu, R. et al. Monolayer 1T-NbSe2 as a Mott insulator. NPG Asia Mater 8, e321 (2016). https://doi.org/10.1038/am.2016.157
This article is cited by
New magneto-polaron resonances in a monolayer of a transition metal dichalcogenide
Scientific Reports (2023)
Charge-density wave associated with higher-order Fermi-surface nesting in monolayer VS2
npj 2D Materials and Applications (2023)
Atomic-scale visualization of chiral charge density wave superlattices and their reversible switching
Nature Communications (2022)
Visualization of edge-modulated charge-density-wave orders in monolayer transition-metal-dichalcogenide metal
Communications Physics (2022)
Robust charge-density wave strengthened by electron correlations in monolayer 1T-TaSe2 and 1T-NbSe2
Nature Communications (2021)